A.Didem et al.
Konstanz, Germany) was marketed as a low-stress flowable base material that can be placed in layers up to 4
mm in thickness without negatively affecting polymerization shrinkage, cavity adaptation or degree of conver-
sion . Also, Tetric EvoCeram Bulk-fill (Ivoclar Vivadent AG, Liechtenstein) was introduced to the market as
a bulk-fill restorative material with the ability to place the restoration with a single increment (up to 4 mm) .
Nowadays a new sonic-activated bulk-fill system (Sonicfill, Kerr Corp, USA/KaVo, Germany) was intro-
duced to the market for posterior bulk restorations. According to the manufacturer’s data, the Sonicfill system is
a unique, sonic-activated bulk-fill system comprised of a specially designed hand piece and a new composite
material in unidose tips. The composite is a combination of flowable and universal composites and incorporates
a highly-filled proprietary resin with special modifiers that react to sonic energy. As sonic energy is applied to
the hand piece with five different levels of flowability, the modifier causes the viscosity to drop (up to 87%), in-
creasing the flowability of the composite. When the sonic energy is stopped, the composite returns to a more
viscous, non-slumping state for carving and contouring. In addition, the manufacturer informs that increased
levels of photoinitiators in the composite material allow a full 5 mm depth of cure in 20 seconds with a 550
light source .
Although the flowable bulk restorations present some advantages for dentists, the number of studies which
have evaluated their properties is still limited -. Research studies on the materials’ physical properties are
clinically relevant. In fact, these kinds of studies are of paramount importance when the material is to be applied
in stress-bearing and clinical uses. The flexural or bending strength is a measure of the fracture resistance of a
material . The compressive strength has an important role in the mastication process  . In the literature
there is very few knowledge about the mechanical properties of new-generation bulk restoration materials. In
addition, the Sonicfill system is the newest material in this area. The aim of this study was to investigate the
flexural and compressive strengths of Sonicfill system and compare the results with other bulk-fill materials
(Surefill SDR, TetricEvoCeram Bulkfill) and a universal posterior composite resin (G-aenial Posterior, GC, Ja-
2. Materials and Methods
The materials used in this study are listed in Table 1.
2.1. Flexural Strength
Ten samples of each material were prepared by the same investigator according to International Standards Or-
ganization (ISO) 4049 specifications (25 × 2 × 2 mm) by using stainless steel split molds and light cured for 20 s
by using a blue light-emitting diode with a 550mW/cm2
light source (Hilux Ledmax 550, Benlioğlu Dental,
Ankara, Turkey) according to the manufacturer’s directions. After polymerization, samples were stored in dis-
tilled water at 37˚C for 24 hours. The flexural tests were performed with a Universal Testing Machine (LF Plus,
LLOYD, Instrument, AmetekInc, England) at a cross-head speed of 1mm/min, with 2 Kn loading force.
2.2. Compressive Strength
Ten cylindrical samples of each material were prepared by the same investigator according to American Dental
Association (ADA) 27 specifications (3 mm diameter × 6 mm height) by using stainless steel split molds and
light cured for 20 s by using a blue light-emitting diode with a 550 mW/cm2
light source (Hilux Ledmax 550).
The universal posterior composite samples were prepared incrementally. The other materials were prepared ac-
cording to the to the manufacturer’s directions for cavities deeper than 4/5 mm height. Samples for compressive
Table 1. The materials used the study.
Material Catagory Brand Name Manufacturer Filler Volume (%) (wt)
Nanohybrid Composite Sonic FillTM
Kerr Corp. USA/KAVO. Germany 83.5%
Nanohybrid Composite TetricEvoCeram Bulk Fill Ivoclar. Vivadent. AG. Liechtenstein 79% - 81%
Flowable Composite SureFil®
Flow Dentsply. Konstanz. Germany 68%
Universal Composite G-aenial Posterior GC Corp. Tokyo. Japan 81%
A.Didem et al.
strength tests were stored in distilled water at 37˚C for 24 hours. The compressive tests were performed with a
Universal Testing Machine (LF Plus, LLOYD, Instrument, Ametek Inc, England) at a cross-head speed for 0.05
Compressive strength and flexural strength tests data’s were subjected to one-way variance analysis and
Kruskal-Wallis tests at a significance level of 0.05.
The mean flexural and compressive strength values (MPa), standard deviations, and statistical results of the ma-
terials are given in Table 2 and Figure 1.
Compressive strength values for the Sonicfill system (316.596 ± 22.23) and universal posterior composite
resin G-aenial (287.9498 ± 28.12) were significantly greater than SDR (218.6399 ± 18.79) and Tetric EvoCeram
(203.6807 ± 26.53) (p < 0.001). No significant difference was observed between the Sonicfill system and uni-
versal posterior composite resin (p = 0.061). No significant difference was observed between SDR and Tetric
EvoCeram (p = 0.518).
Although the greatest flexural strength values were observed for the Sonicfill system (163.47 ± 49.74), no sta-
tistically significant differences were observed among all groups (G-aenial: 158.12 ± 11.92 SDR: 142.04 ±
27.89, Tetric EvoCeram: 135.16 ± 31.16) (p > 0.001).
Direct posterior restorations play a significant role in dentistry. But achieving predictable and successful out-
comes remains a main concern for practitioners, due to technique sensitivity and the numerous steps required for
proper placement. In addition, several negative effects in resin-based composite restorations are frequently con-
nected to polymerization shrinkage stress  . Filling all of a tooth preparation with a composite at one time
Table 2. Mean compressive and flexural strength values of the materials tested.
Groups Compressive Strength Flexural Strength
N Mean (MPa) Std. Dev. Mean (MPa) Std. Dev.
Sonicfill System 10 316.1596a
22.23 163.47 49.74
SDR 10 218.6399b
18.79 142.04 27.89
Tetric EvoCeram 10 203.6807b
26.53 135.16 31.16
G-aenial 10 287.9498a
28.12 158.12 11.92
Same lower cases in the same column mean no statistically significant difference (p < 0.001).
Figure 1. Comparison of the compressive and flexural strength values of the materials tested.
Sonicfill System SDR TetricEvoCeram G-aenial
A.Didem et al.
has obvious advantages for both patients and practitioners .
Although a new category of bulk-fill resin-based composites have been introduced, there are very few studies
investigating the clinical and laboratory success of these materials   -. The manufacturers claimed
that bulk-fill materials can achieve a depth of cure of 6 mm. In this context, the studies were focused on the po-
lymerization shrinkage , depth of cure , marginal quality , shrinkage stress , and surface morphol-
ogy , especially of SDR. In one study the flexural strength of SDR was investigated . The Sonicfill system
is a new development in this area and in the limitation of our knowledge this is the first study in which the main
physical properties of either the Sonicfill system or new bulk-fill materials were investigated. This study com-
pared the compressive and flexural strengths of three resin based composites that, according to their manufac-
turers, are capable of being placed in bulk.
The performance of biomaterials is most often evaluated using laboratory tests. Restorative materials and
teeth are generally subjected to both compressive and flexural forces, so flexural and compressive strength tests
are very important to test and determine the mechanical properties of materials  . The compressive strength
has an important role in the mastication process since several of the masticatory forces are of a compressive na-
ture . In addition, a material’s fracture-related properties are usually determined by flexural strength testing
and are especially important if the material is used for Class I, II, or IV cavities, which are usually subjected to
high forces . For screening of resin-based materials, the flexural strength test is one of the mechanical prop-
erties selected by ISO . Similarly, the ADA established guidelines for in-vitro tests of resin-based materials
. In this study, the specimen dimensions were prepared according to ISO 4049 specifications for a flexural
strength test and ADA 27 specifications for a compressive strength test.
In the study, a low-stress flowable base material (SDR that can be placed in layers up to 4 mm), a bulk-fill
composite resin (Tetric Evo Ceram), a universal posterior composite (G-aenial), and the Sonicfill system were
compared. The ISO has set 80 MPa as the minimum flexural strength for polymer-based filling and restorative
materials claimed suitable and acceptable for restorations involving outer occlusal surfaces . Accordingly,
our results showed that all of the tested materials can be used in occlusal areas. Although no statistically signifi-
cant differences were observed among all groups, the greatest flexural strength values were observed for the
Sonicfill system. Additionally, the present study demonstrated that compressive strength values for the Sonicfill
system and G-aenial were significantly greater than SDR and Tetric EvoCeram.
It is generally assumed that the higher the filler loading, the higher the composite mechanical properties . It
is known that the average filler content’s of flowables vary from 45% to 65% by weight. In this context, the
Sonicfill system, with highest flexural and compressive strength values (163.47 MPa, 316.15 MPa, respectively),
is also the material with the greatest filler loading (83.5%), as seen in Table 1. Similarly, Tetric Evo Ceram and
SDR, which present the lowest strength values for both flexural and compressive tests, also have the minimum
amount of filler loadings (79% - 81%, and 68%, respectively).
These results can also be explained by the working principle of the Sonicfill system. The composite used in
this system is a combination of flowable and universal composites and incorporates a highly-filled proprietary
resin with special modifiers that react to sonic energy. As sonic energy is applied through the hand piece, the
modifier causes the viscosity to drop (up to 87%), increasing the flowability of the composite. When the sonic
energy is stopped, the composite returns to a more viscous, non-slumping state . In this context, the Sonicfill
system cannot be classified as a flowable composite. The flowability is adjusted by the practitioner through the
hand piece with five levels of flowability and when the sonic activation stopped, the material becomes similar to
a universal composite structure. However, these tests need further clinical observations because occlusal forces
may influence flexural and compressive strengths.
Physical property studies are accepted methods to evaluate resin materials. The present study showed that all
of the tested materials are suitable and acceptable for restorations involving outer occlusal surfaces. The Soni-
cfill system created the greatest mechanical properties. Moreover, the bulk-fill technology has obvious advan-
tages: 1) fewer voids may be present in the mass of the material, since all of it is placed at one time; 2) the tech-
nique would be faster than placing numerous increments if curing times were identical; 3) It may be easier than
numerous increments  . On the other hand, there are many questions in the minds of dentists about bulk-
fill technology because there are very few published data. Therefore, the clinical success will only be discovered
after long periods of use by general practitioners. Further studies evaluating the long-term clinical success of
bulk-fill resin based composites are needed.
A.Didem et al.
It can be concluded that the physical properties of the Sonicfill system demonstrated results for flexural strength
tests comparable to universal composite, whereas the compressive strength tests revealed superior results to the
other bulk-fill materials. Due to the ability to place restorations with a single increment (up to 5 mm) and ease of
use, by further in-vitro and in-vivo studies, the Sonicfill system may be an alternative for posterior restorations.
 Salerno, M., Derchi, G., Thorat, S., Ceseracciu, L., Ruffilli, R. and Barone, A.C. (2011) Surface Morphology and Me-
chanical Properties of New-Generation Flowable Resin Composites for Dental Restoration. Dental Materials, 27,
 Ozel, E., Korkmaz, Y., Attar, N. and Karabulut, E. (2008) Effect of One-Step Polishing Systems on Surface Roughness
of Different Flowable Restorative Materials. Dental Materials Journal, 27, 755-764.
 Ilie, N. and Hickel, R. (2011) Investigations on a Methacrylate-Based Flowable Composite Based on the SDR™
Technology. Dental Materials, 27, 348-355. http://dx.doi.org/10.1016/j.dental.2010.11.014
 Roggendorf, M.J., Krämer, N., Appelt, A., Naumann, M. and Frankenberger, R. (2011) Marginal Quality of Flowable
4-mm Base vs. Conventionally Layered Resin Composite. Journal of Dentistry, 39, 643-647.
 Boaro, L.C., Gonçalves, F., Guimarães, T.C., Ferracane, J.L., Versluis, A. and Braga, R.R. (2010) Polymerization
Stress, Shrinkage and Elastic Modulus of Current Low-Shrinkage Restorative Composites. Dental Materails, 26,
 Heintze, S.D. and Zimmerli, B. (2011) Relevance of in Vitro Tests of Adhesive and Composite Dental Materials. A
Review in 3 Parts. Part 3: In Vitro Tests of Adhesive Systems. Schweiz Monatsschr Zahnmed, 121, 1024-1040.
 Silva, C.M. and Dias, K.R. (2009) Compressive Strength of Esthetic Restorative Materials Polymerized with Quartz-
Tungsten-Halogen Light and Blue LED. Brazillian Dental Journal, 20, 54-57.
 Gömeç, Y., Dörter, C., Dabanoglu, A. and Koray, F. (2005) Effect of Resin-Based Material Combination on the Com-
pressive and the Flexural Strength. Journal of Oral Rehabilitation, 32, 122-127.
 Uçtaşli, M.B., Bala, O. and Güllü, A.V. (2004) Surface Roughness of Flowable and Packable Composite Resin Materi-
als after Finishing with Abrasive Discs. Journal of Oral Rehabilitation, 31, 1197-1202.
 Christensen, G.J. (2012) Advantages and Challenges of Bulk-Fill Resins. Clinicians Report, 5, 1-5.
 Ilie, N. and Hickel, R. (2009) Investigations on Mechanical Behaviour of Dental Composites.Clinical Oral Inves-
tigations, 13, 427-438. http://dx.doi.org/10.1007/s00784-009-0258-4
 Burgess, J. and Cakir, D. (2010) Comparative Properties of Low-Shrinkage Composite Resins. Compendium of Conti-
nuing Education in Dentistry, 31, 10-15.
 Czasch, P. and Ilie, N. (2012) In Vitro Comparison of Mechanical Properties and Degree of Cure of Bulk Fill Com-
posites. Clinical Oral Investigations, 17, 227-235.
 Ersoy, M., Civelek, A., L’Hotelier, E., Say, E.C. and Soyman, M. (2004) Physical Properties of Different Composites.
Dental Materials Journal, 23, 278-283. http://dx.doi.org/10.4012/dmj.23.278
 International Standard ISO 4049 (2000) Polymer-Based Filling, Restorative and Luting Materials. Technical Commit-
tee 106-Dentistry. International Standards Organization, Geneva.
 Attar, N., Tam, L.E. and McComb, D. (2003) Flow, Strength, Stiffness and Radiopacity of Flowable Resin Composites.
Journal of Canadian Dental Associations, 69, 516-521.